Synthesis and characterization of titanium complex with a dithiolate ligand for green LCD color filter dyes
© Shin et al.; licensee Springer. 2012
Received: 12 July 2012
Accepted: 3 October 2012
Published: 21 November 2012
Three green compounds for color filter dyes based on bis(cyclopentadienyl) titanium complexes including dithiolate ligand were synthesized. Physical properties by the change of the substitution groups of the synthesized materials were systematically examined. UV-visible absorption spectrum of the synthesized materials showed maximum absorbing wavelengths of 427 to 430 nm and 632 to 635 nm in solution state, and 434 to 438 nm and 637 to 651 nm in film state, indicating green and black colors. It was observed that the extinction coefficient values (log ε) of all the synthesized materials are very high at 4.0 or above. In addition, it was shown that since the Td values of three synthesized materials show thermal stability higher than 240°C, they possess high potential to be applied as dyes for LCD color filter and black matrix addictive.
KeywordsBis(cyclopentadienyl) titanium complex Pigment Dyes Molar extinction coefficiency Color filter Black matrix additive Ligand-to-ligand charge transfer.
Recently, thin-film transistor liquid crystal display (TFT LCD) panels have become increasingly important in the flat display panel industry . Among major parts in TFT LCD panels, red, green, and blue (RGB) color filters are a very essential component for rendering full color images in TFT LCD panels. Various types of dyes and pigments for RGB color filters have been extensively developed and commercially utilized in manufacturing color filters of TFT LCD panels. So far, a wide range of blue and red color filter materials has been developed. However, a limited number of dyes and pigments for pure green color filters have been introduced because it is difficult to synthesize dye and pigment molecules which simultaneously absorb the light of both violet (<450 nm) and red (>600 nm) regions, but not that of around 500-nm region.
In order to manufacture a color filter for large-sized TFT LCD panels, the ink-jet printing technology has been extensively used since it affords a facile and economic production process. To apply ink-jet printing technology, dye-type color filter materials are preferred to pigment-type compounds because dye color filters are cheaper and have an easy control of fabrication process and a superior chromatic property, whereas the ink-jet nozzle is often blocked by insoluble pigment particles. However, dye-type color filter materials are needed to overcome the poor thermal stability for the high durability of TFT LCDs.
1H-NMR spectra were recorded on Avance III 300 (Bruker BioSciences Korea Co. Ltd., Seoul, South Korea). Fast atom bombardment (FAB) mass spectra were recorded by JMS-AX505WA, HP5890 series II (Jeol Korea Ltd., Seoul, South Korea). The optical absorption spectra were obtained by HP 8453 UV-vis-NIR spectrometer (Hewlett-Packard Asia Pacific Ltd., Singapore). Degradation temperatures (Td) of the compounds were measured by thermogravimetric analysis (TGA) using a SDP-TGA2960 (TA Instruments, DE, USA).
Synthesis of tetraethylammonium bis(1,3-dithiole-2-thione-4,5-dithiol)zincate (ZnCS2)
Three-liter round flask was charged with sodium shaving (2.3 g, 0.1 mol) via a solid addition funnel and, after reassembly, the apparatus was flushed with N2 for 5 min and placed in ice-water bath. Carbon disulfide (18 ml, 0.3 mol) was introduced into the flask through the dropping funnel. After which, the dropping funnel was immediately loaded with 20 ml dimethylformamide (DMF), the system was closed, and N2 atmosphere was maintained throughout the reaction. The DMF was added dropwise with stirring over 1 hr, during which, a red color appears. Upon completion of the addition, the temperature of the reaction mixture was allowed to warm to room temperature. The mixture was stirred overnight, during which time it becomes increasingly deep red. The reaction mixture was visually inspected for residual sodium. As a precaution, ice was added to the cooling bath and 40 ml methanol and 50 ml deionized water, which is degassed by applying vacuum, were then added rapidly through the dropping funnel. A solution of zinc chloride (2 g, 0.15 mol) in a mixture of 40-ml concentrated ammonium hydroxide and 50 ml of methanol was then added through the dropping funnel. A solution of tetraethylammonium bromide (5.3 g 0.025 mol) in 25 ml of deionized water was added dropwise via the dropping funnel with vigorous stirring over at least 1 h, and the solution was stirred overnight . A large amount of red precipitate develops in the flask overnight. This salt was collected by solution on a Buchner funnel and was washed immediately with 50 ml of deionized water, then with 40 ml portion of isopropyl alcohol until the filtrate is colorless, and finally once with 20 ml of diethyl ether. After completion of the reaction, the solvent was evaporated under vacuum, and the product was extracted with dichloromethane (CH2Cl2). The CH2Cl2 solution was washed with water and dried with magnesium sulfate anhydrous. The solvent was evaporated to give ZnCS2 as red solid, which was recrystallized from CH2Cl2 and hexane (yield 81%).
Synthesis of Bis(cyclopentadienyl)titanium complex (CPTiCS)
Treatment of Bis(cyclopentadienyl)Titanium(IV) dichloride (1g, 4mmol) with 0.6 equiv of ZnCS2 in refluxing tetrahydrofuran(THF) resulted in a color change red to green. After 4 h, the cooled solution was filtered through a silica gel, concentrated, and diluted with hexane to afford deep green crystals of CP2TiCS  (yield 40%). 1H-NMR (300 MHz, DMSO) 6.12 (s, 10H). C13H10S5Ti, found C, 42.73; H, 2.62; S, 42.87; calculated C, 41.70; H, 2.69; S, 42.82; FAB-mass: 374 m/z.
Synthesis of bis(ethylcyclopentadienyl)titanium complex (ECPTiCS)
Treatment of bis(ethylcyclopentadienyl)titanium(IV) dichloride (0.5 g, 1.6mmol) with 0.6 equivalents of ZnCS2 in refluxing THF resulted in a color change from red to green. After 6 h, the cooled solution was filtered through a silica gel, concentrated, and diluted with hexane to afford black crystals of ECP2TiCS (yield 41.8%). 1H-NMR (300 MHz, DMSO), 6.15 (d, 8H), 2.36 (m, 4H), 1.01 (t, 6H). C17H18S5Ti, found C, 47.52; H, 4.24; S, 37.17; calculated C, 47.43; H, 4.21; S, 37.24; FAB-mass 430 m/z.
Synthesis of bis(tetrabutlycyclopentadienyl)titanium complex (TCPTiCS)
Treatment of bis(tetrabutlycyclopentadienyl)titanium(IV) dichloride (0.9 g, 2.5 mmol) with 0.6 equivalents of ZnCS2 in refluxing THF resulted in a color change from red to green. After 4 h, the cooled solution was filtered through silica gel, concentrated, and diluted with hexane to afford deep green crystals of TCP2TiCS (yield 40%). 1H-NMR (300 MHz, DMSO) 6.13 (d, 8H), 1.12 (s, 18H). C21H26S5Ti, found C, 51.89; H, 5.49; S, 32.98; calculated C, 51.83; H, 5.39; S, 32.95; FAB-mass 486 m/z.
Solubility of ECPTiCS, bis(cyclopentadienyl)titanium complex (CPTiCS), and TCPTiCS
For solubility test, 0.1 g of compound and 0.4 g of PGMEA were mixed and stirred for 20 h. After stirring, syringe filter (membrane material: Teflon) was used for filtering. Then, the weight of the specimen on the membrane was measured by the difference before/after filtering .
Results and discussion
Optical properties of synthesized materials
Solution UVmax (nm)
Film UVmax (nm)
In ligand-metal-ligand complex synthesized in this study, dithiolate ligand was used as π-electron donor, and bis(cyclopentadienyl) group was used as π-electron acceptor. Thiolate unit which is electron rich and bis(cyclopentadienyl) unit which is relatively electron lacking were attached on titanium(IV) center metal in one molecule. This induces intramolecular ligand-to-ligand charge transfer (LLCT) [5, 6]. As a result, the light of blue and red area is absorbed, and it eventually shows green-colored UV-absorption spectra  (Figure 5).
The absorption band in the range of 400 to 500 nm (blue absorption region) and 600 to 800 nm (red absorption region) is attributed to the π-π* transition of 1,3-dithiole-2-thione-4,5-dithiolato (dmit) ligand and ‘intramolecular’ LLCT, respectively [7, 8]. Regarding the LLCT process, the charge transfer (CT) band is presumably originated from electron-rich dmit ligand to the cyclopentadieneyl electron acceptor which is also often observed in the metal complex system containing both a dmit ligand as an electron donor and a bypyridine ligand as a π-electron acceptor [5–7].
The three synthesized dyes were measured for ε under the conditions of THF solvent. As the result, all synthesized substances showed high log scale ε value of over 4.0. The properties of materials with high ε values and absorbing 300 to 800 nm at the same time confirmed that it can be used not only as green dye for LCD color filter but also as the additive substance used for black matrix. As mentioned the above, the absorption bands of Ti complex dyes mainly originated from a mixture of π-π* transition and LLCT, owing to the dmit ligand. In general, it is well known that π-π* and CT transitions have high molar extinction coefficients (>10,000 L/mol·cm), leading to the intense absorption bands, whereas n-π* and d-d transitions exhibit a low molar extinction coefficients, ε = 10 to 100 and ε = 5 to 500 L/mol·cm, respectively [5–8].
Optical and thermal properties of synthesized materials
Solubility (PGMEA) (%)
A new class of green dyes based on bis(cyclopentadienyl) titanium complexes, CPTiCS, ECPTiCS, and TCPTiCS, were designed and synthesized for LCD color filters. All prepared green dyes were soluble in a common color filter solvent, PGMEA, (over 10 wt% of solubility) and exhibited distinctive absorption bands around at 430 nm and 630 nm with a high molar extinction coefficient (log ε > 4.0) owing to the π-π* transition and ligand-to-ligand charge transfer (LLCT), respectively. In addition they showed a high thermal stability with 5% weight-loss temperature beyond 241°C and their spin-coated films had no significant change of absorption spectra after heating treatment at 200°C for 30 min.
HS is a masters degree student on Organic Material Chemistry. YP is a Ph.D. degree holder on Organic Material Chemistry and is currently a postdoctoral fellow. SK is a masters degree student on Organic Material Chemistry. BKA is a Chemistry professor and is majoring in Analytical Chemistry. JP is a full professor on Organic Material Chemistry. He is also a director of Display Research Center of the Catholic University in South Korea.
This work was supported by the National Research Foundation of Korea (NRF) grant funded by the Korean government (MEST) (grant no. 2012001846).
- Sabnis RW: Color filter technology for liquid crystal displays. Displays 1999, 20: 119. 10.1016/S0141-9382(99)00013-XView ArticleGoogle Scholar
- Hansen TK, Becher J, Jorgensen T, Sukumar Varma K, Khedekar R, Cava MP: 4,5-Dibenzoyl-1,3-dithiole-1-thione. Organic Synth 1998, 9: 203.Google Scholar
- Yang X, Rauchfuss TB, Wilson SR: An organometallic route to binary carbon sulfides the structure of C6S12. J Am Chem Soc 1989, 111: 3465. 10.1021/ja00191a072View ArticleGoogle Scholar
- Choi J, Se Hun K, Lee W, Yoon C, Kim JP: Synthesis and characterization of thermally stable dyes with improved optical properties for dye-based LCD color filters. New J Chem 2012, 36: 812. 10.1039/c2nj20938aView ArticleGoogle Scholar
- Miller TR, Dance IG: Reactions of dithiolene complexes with amines. II. Formation and properties of mixed-ligand dithiolene. Alpha.-diimine complexes of nickel. J Am Chem Soc 1973, 95: 6970. 10.1021/ja00802a017View ArticleGoogle Scholar
- Vogler A, Kunkely H: Photooxidation of (2,2‘-bipyridine)(3,4-toluenedithiolato)platinum(II) following ligand-to-ligand and charge-transfer excitation. J Am Chem Soc 1981, 103: 1559. 10.1021/ja00396a045View ArticleGoogle Scholar
- Matsubayashi G-E, Hirao M, Tanaka T: Spectroscopic and electrical properties of the PtIIS2N2 type complexes and their iodine-doped analogs. Inorg Chim Acta 1988, 144: 217. 10.1016/S0020-1693(00)86289-1View ArticleGoogle Scholar
- Steimecke G, Sieler H, Krimse R, Hoyer B: 1.3-dithiol-2-thion-4.5-dithiolat aus schwefelkohlenstoff und alkalimetall. Phosphorous Sulfur 1979, 7: 49. 10.1080/03086647808069922View ArticleGoogle Scholar
- Choi J, Lee W, Sakong C, Yuk S, Park JS, Kim JP: Facile synthesis and characterization of novel coronene chromophores and their application to LCD color filters. Dye Pigment 2012, 94: 34. 10.1016/j.dyepig.2011.11.009View ArticleGoogle Scholar
- Kim YD, Kim JP, Kwon OS, Cho IH: The synthesis and application of thermally stable dyes for ink-jet printed LCD color filters. Dye Pigment 2009, 81: 45. 10.1016/j.dyepig.2008.09.006View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.